This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
Designation: C109/C109M − 16a
Standard Test Method for
Compressive Strength of Hydraulic Cement Mortars (Using 2-in. or [50-mm] Cube Specimens) 1 This standard is issued under the ﬁxed designation C109/C109M; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revis revision. ion. A number in parentheses parentheses indicates the year of last reapproval. reapproval. A superscript epsilon (´) indicates an editorial change since the last revision or reapproval. This standard has been approved for use by agencies of the U.S. Department of Defense.
1. Sco Scope* pe*
2. Referenc Referenced ed Documents
1.1 This test method covers determination determination of the compressivee st siv stre reng ngth th of hy hydr drau aulic lic ce ceme ment nt mo mort rtar ars, s, us usin ing g 22-in in.. or [50-mm] [50-m m] cube specime specimens. ns. NOTE 1—Test Method C349 Method C349 provides provides an altern alternative ative procedure procedure for this determination (not to be used for acceptance tests).
1.2 This test method covers covers the application application of the test using either inch-pound or SI units. The values stated in either SI units uni ts or inch inch-po -pound und units are to be reg regard arded ed sep separa arately tely as standard. Within the text, the SI units are shown in brackets. The values stated in each system may not be exact equivalents; equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in nonconformance with the standard. 1.3 Values in SI units shall be obtained by measurement measurement in SI uni units ts or by app approp ropria riate te con conver versio sion, n, usi using ng the Rule Ruless for Conver Con versio sion n and Rou Roundi nding ng giv given en in IEE IEEE/A E/ASTM STM SISI-10, 10, of measurements made in other units. standard d doe doess not purport purport to add addre ress ss all of the 1.4 This standar safet sa fetyy co conc ncer erns ns,, if an anyy, as asso socia ciate ted d wi with th its us use. e. It is th thee responsibility of the user of this standard to establish appro priate safety and health practices and determine the applicability of regulatory limitations prior to use. (Warning—Fresh hydraulic hydra ulic cement cementitious itious mixtures mixtures ar aree causti causticc and may cause chemical burns to skin and tissue upon prolonged exposure. 2) intern ernati ationa onall sta standa ndard rd was dev develo eloped ped in acc accor or-1.5 This int dance with internationally recognized principles on standardizatio iza tion n es esta tabl blis ishe hed d in th thee De Decis cisio ion n on Pr Prin incip ciple less fo forr th thee Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2.1 ASTM Standards: 3 C91 Speciﬁcation C91 Speciﬁcation for Masonry Cement C114 Test Meth Methods ods for Che Chemic mical al Ana Analys lysis is of Hyd Hydrau raulic lic Cement C150 Speciﬁcation C150 Speciﬁcation for Portland Cement C230/C230M Speciﬁcation C230/C230M Speciﬁcation for Flow Table for Use in Tests of Hydraulic Cement C305 Practice C305 Practice for Mechanical Mixing of Hydraulic Cement Pastes and Mortars of Plastic Consistency C349 Test C349 Test Method for Compressive Strength of HydraulicCement Ceme nt Mor Mortar tarss (Us (Using ing Por Portion tionss of Pri Prisms sms Bro Broken ken in Flexure) C511 Spe Speciﬁc ciﬁcatio ation n for Mix Mixing ing Roo Rooms, ms, Moi Moist st Cabi Cabinets nets,, Mois Mo istt Ro Room oms, s, an and d Wat ater er St Stor orag agee Tan anks ks Us Used ed in th thee Testing of Hydraulic Cements and Concretes C595 Speciﬁcation C595 Speciﬁcation for Blended Hydraulic Cements C618 Speciﬁcation for Coal Fly Ash and Raw or Calcined C618 Natural Pozzolan for Use in Concrete C670 Practice C670 Practice for Preparing Precision and Bias Statements for Test Methods for Construction Materials C778 Speciﬁcation C778 Speciﬁcation for Standard Sand C989 Speciﬁcation C989 Speciﬁcation for Slag Cement for Use in Concrete and Mortars C1005 Speciﬁcation C1005 Speciﬁcation for Reference Masses and Devices for Determi Dete rminin ning g Mas Masss and Volu Volume me for Use in the Phy Physic sical al Testing of Hydraulic Cements C1157 Perfor C1157 Performance mance Speciﬁ Speciﬁcation cation for Hydr Hydraulic aulic Cement C1328 Speciﬁcation C1328 Speciﬁcation for Plastic (Stucco) Cement C1329 Speciﬁcation C1329 Speciﬁcation for Mortar Cement C1437 Test C1437 Test Method for Flow of Hydraulic Cement Mortar E4 Practices E4 Practices for Force Veriﬁcation of Testing Machines 2.2 IEEE/ASTM Standard:3 IEEE/ASTM IEEE/A STM SI-10 Stan Standar dard d for Use of the Int Intern ernatio ational nal System of Units (SI): The Modern Metric System
This test method is under the jurisdiction of ASTM Committee C01 C01 on on Cement and is the direct respo responsibil nsibility ity of Subco Subcommitte mmitteee C01.27 C01.27 on on Strength. Current Curre nt editio edition n approv approved ed March 1, 2016. Published Published April 2016. Origin Originally ally approved in 1934. Last previous edition approved in 2016 as C109/C109M – 16. DOI: 10.1520/C0109_C0109M-16A. 2 See the section on Safety, Manual of Cement Testing, Annual Book of ASTM Standards, Vol 04.01.
3 For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected]
For Annual Book of ASTM Standards volume information, refer to the standard’s Document Summary page on the ASTM website.
*A Summary of Changes section appears at the end of this standard Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959. United States
Copyright by ASTM Int'l (all rights reserved); Thu Sep 14 12:25:02 EDT 2017 1 Downloaded/printed by Robb Dibble (Dibble Engineers, Inc) pursuant to License Agreement. No further reproductions authorized.
C109/C109M − 16a 3. Summary of Test Method 3.1 The mortar used consists of 1 part cement and 2.75 parts of sand proportioned by mass. Portland or air-entraining portland cements are mixed at speciﬁed water/cement ratios. Water content for other cements is that sufficient to obtain a ﬂow of 110 6 5 in 25 drops of the ﬂow table. Two-inch or [50-mm] test cubes are compacted by tamping in two layers. The cubes are cured one day in the molds and stripped and immersed in lime water until tested. 4. Signiﬁcance and Use 4.1 This test method provides a means of determining the compressive strength of hydraulic cement and other mortars and results may be used to determine compliance with speciﬁcations. Further, this test method is referenced by numerous other speciﬁcations and test methods. Caution must be exercised in using the results of this test method to predict the strength of concretes. 5. Apparatus 5.1 Weights and Weighing Devices, shall conform to the requirements of Speciﬁcation C1005. The weighing device shall be evaluated for precision and accuracy at a total load of 2000 g. 5.2 Glass Graduates, of suitable capacities (preferably large enough to measure the mixing water in a single operation) to deliver the indicated volume at 20°C. The permissible variation shall be 62 mL. These graduates shall be subdivided to at least 5 mL, except that the graduation lines may be omitted for the lowest 10 mL for a 250-mL graduate and for the lowest 25 mL of a 500-mL graduate. The main graduation lines shall be circles and shall be numbered. The least graduations shall extend at least one seventh of the way around, and intermediate graduations shall extend at least one ﬁfth of the way around. 5.3 Specimen Molds, for the 2-in. or [50-mm] cube specimens shall be tight ﬁtting. The molds shall have not more than three cube compartments and shall be separable into not more than two parts. The parts of the molds when assembled shall be positively held together. The molds shall be made of hard metal not attacked by the cement mortar. For new molds the Rockwell hardness number of the metal shall be not less than 55 HRB. The sides of the molds shall be sufficiently rigid to prevent spreading or warping. The interior faces of the molds shall be plane surfaces and shall conform to the tolerances of Table 1.
5.3.1 Cube molds shall be checked for conformance to the design and dimensional requirements of this test method at least every 2½ years. 5.4 Mixer, Bowl and Paddle, an electrically driven mechanical mixer of the type equipped with paddle and mixing bowl, as speciﬁed in Practice C305. 5.5 Flow Table and Flow Mold, conforming to the requirements of Speciﬁcation C230/C230M. 5.6 Tamper, a nonabsorptive, nonabrasive, nonbrittle material such as a rubber compound having a Shore A durometer hardness of 80 6 10 or seasoned oak wood rendered nonabsorptive by immersion for 15 min in paraffin at approximately 392°F or [200°C], shall have a cross section of 0.5 ( 60.06) by 1-in (60.06) [13 ( 61.6) by 25 ( 61.6) mm] and a length of 5 to 6 in. or [120 to 150 mm]. The tamping face shall be ﬂat and at right angles to the length of the tamper. 5.6.1 Tampers shall be checked for conformance to the design and dimensional requirements of this test method at least every six months. NOTE 2—Each day that the tamper is used a visual inspection should conﬁrm that the end is ﬂat and at a right angle to the long axis of the tamper. Rounded or peeling tampers should not be allowed for use.
5.7 Trowel, having a steel blade 4 to 6 in. [100 to 150 mm] in length, with straight edges. 5.8 Moist Cabinet or Room, conforming to the requirements of Speciﬁcation C511. 5.9 Testing Machine, either the hydraulic or the screw type, with sufficient opening between the upper bearing surface and the lower bearing surface of the machine to permit the use of verifying apparatus. The load applied to the test specimen shall be indicated with an accuracy of 61.0 %. If the load applied by the compression machine is registered on a dial, the dial shall be provided with a graduated scale that can be read to at least the nearest 0.1 % of the full scale load ( Note 3). The dial shall be readable within 1 % of the indicated load at any given load level within the loading range. In no case shall the loading range of a dial be considered to include loads below the value that is 100 times the smallest change of load that can be read on the scale. The scale shall be provided with a graduation line equal to zero and so numbered. The dial pointer shall be of sufficient length to reach the graduation marks; the width of the end of the pointer shall not exceed the clear distance between the smallest graduations. Each dial shall be equipped with a zero adjustment that is easily accessible from the outside of the
TABLE 1 Permissible Variations of Specimen Molds Parameter Planeness of sides Distance between opposite sides Height of each compartment Angle between adjacent facesA
2-in. Cube Molds New In Use